Presentation on theme: "Introduction to X-Ray Powder Diffraction Data Analysis"— Presentation transcript:
1 Introduction to X-Ray Powder Diffraction Data Analysis Scott A Speakman, Ph.D.Center for Materials Science and Engineering at MIT
2 An X-ray diffraction pattern is a plot of the intensity of X-rays scattered at different angles by a sampleThe detector moves in a circle around the sampleThe detector position is recorded as the angle 2theta (2θ)The detector records the number of X-rays observed at each angle 2θThe X-ray intensity is usually recorded as “counts” or as “counts per second”To keep the X-ray beam properly focused, the sample will also rotate.On some instruments, the X-ray tube may rotate instead of the sample.X-ray tubeDetectorw2qsamplePosition [°2Theta] (Cu K-alpha)3540455055Intensity (Counts)500010000Slide ‹#› of 20Scott A Speakman, Ph.D.
3 Each “phase” produces a unique diffraction pattern Position [°2Theta] (Cu K-alpha)152025303540QuartzCristobaliteGlassA phase is a specific chemistry and atomic arrangement.Quartz, cristobalite, and glass are all different phases of SiO2They are chemically identical, but the atoms are arranged differently.As shown, the X-ray diffraction pattern is distinct for each different phase.Amorphous materials, like glass, do not produce sharp diffraction peaks.The X-ray diffraction pattern is a fingerprint that lets you figure out what is in your sample.Slide ‹#› of 20Scott A Speakman, Ph.D.
4 The diffraction pattern of a mixture is a simple sum of the diffraction patterns of each individual phase.Position [°2Theta] (Copper (Cu))152025303540MixturePosition [°2Theta] (Cu K-alpha)152025303540QuartzCristobaliteGlassFrom the XRD pattern you can determine:What crystalline phases are in a mixtureHow much of each crystalline phase is in the mixture (quantitative phase analysis, QPA, is covered in another tutorial)If any amorphous material is present in the mixtureSlide ‹#› of 20Scott A Speakman, Ph.D.
5 Qualitative Analysis of XRD Data Slide ‹#› of 20Scott A Speakman, Ph.D.
6 Experimental XRD data are compared to reference patterns to determine what phases are present The reference patterns are represented by sticksThe position and intensity of the reference sticks should match the dataA small amount of mismatch in peak position and intensity is acceptable experimental errorSlide ‹#› of 20Scott A Speakman, Ph.D.
7 Specimen Displacement Error will cause a small amount of error in peak positions Peaks that are close together should be shifted the same direction and by the same amountThe peak shift follows a cosθ behavior, so peak shift might change direction over a large angular rangeSpecimen displacement is a systematic peak position error due to misalignment of the sample.The direction and amount of peak shift will vary as −2𝑠 cos 𝜃 𝑅Slide ‹#› of 20Scott A Speakman, Ph.D.
8 Most diffraction data contain K-alpha1 and K-alpha2 peak doublets rather than just single peaks The k-alpha1 and k-alpha2 peak doublets are further apart at higher angles 2thetaThe k-alpha1 peaks always as twice the intensity of the k-alpha2At low angles 2theta, you might not observe a distinct second peakSlide ‹#› of 20Scott A Speakman, Ph.D.
9 The experimental data should contain all major peaks listed in the reference pattern Minor reference peaks could be lost in the background noise, so it may be acceptable if they are not observedIf a major reference peak is not observed in the data, then that is not a good matchThis is an example of a bad match between the data and the reference patternSlide ‹#› of 20Scott A Speakman, Ph.D.
10 Each different phase produces a different combination of peaks. The X-ray diffraction pattern is a sum of the diffraction patterns produced by each phase in a mixtureNote that rutile and anatase are both polymorphs of TiO2Each different phase produces a different combination of peaks.Slide ‹#› of 20Scott A Speakman, Ph.D.
11 You cannot guess the relative amounts of phases based upon the relative intensities of the diffraction peaksThe pattern shown above contains equal amounts of TiO2 and Al2O3The TiO2 pattern is more intense because TiO2 diffracts X-rays more efficientlyWith proper calibration, you can calculate the amount of each phase present in the sampleSlide ‹#› of 20Scott A Speakman, Ph.D.
12 Diffraction peak broadening may contain information about the sample microstructure Peak broadening may indicate:Smaller crystallite size in nanocrystalline materialsMore stacking faults, microstrain, and other defects in the crystal structureAn inhomogeneous composition in a solid solution or alloyHowever, different instrument configurations can change the peak width, tooThese patterns show the difference between bulk ceria (blue) and nanocrystalline ceria (red)These patterns show the difference between the exact same sample run on two different instruments.When evaluating peak broadening, the instrument profile must be considered.Slide ‹#› of 20Scott A Speakman, Ph.D.
13 Quantitative Analysis of XRD Data Slide ‹#› of 20Scott A Speakman, Ph.D.
14 Diffraction peak positions can be used to calculated unit cell dimensions degd= Ådegd= ÅThe unit cell dimensions can be correlated to interatomic distancesAnything the changes interatomic distances- temperature, subsitutional doping, stress- will be reflected by a change in peak positionsSlide ‹#› of 20Scott A Speakman, Ph.D.
15 To calculate unit cell lattice parameters from the diffraction peak positions Convert the observed peak positions, °2theta, into dhkl values using Bragg’s Law:Determine the Miller indices (hkl) of the diffraction peaks from the published reference patternIf you do not have access to a reference pattern that identifies (hkl) then you will need to index the pattern to determine the (hkl)Use the d*2 equation to calculate the lattice parametersMost analysis programs contain an unit cell refinement algorithm for numerically solving the lattice parametersThese programs can also calculate and correct for peak position error due to specimen displacement𝑑 ℎ𝑘𝑙 = λ 2 sin θSlide ‹#› of 20Scott A Speakman, Ph.D.
16 The diffraction peak width may contain microstructural information Width=0.007 radXS ~ 19 nmWidth=0.002 radXS> 90 nmSize = 𝐾λ 𝑊𝑖𝑑𝑡ℎ∗ cos 𝜃For quantitative analysis, you want to use many peaks over a long range.Nanocrystallite size will produce peak broadening that can be quantifiedOnce the crystallite size is larger than a maximum limit, the peak broadening cannot be quantified. This creates an upper limit to the crystallite size that can be calculated.The upper limit depends on the resolution of the diffractometer.Non-uniform lattice strain and defects will also cause peak broadeningCareful evaluation is required to separate all of the different potential causes of peak broadeningSlide ‹#› of 20Scott A Speakman, Ph.D.
17 The weight fraction of each phase can be calculated if the calibration constant is known The calibration constants can be determined:By empirical measurements from known standardsBy calculating them from published reference intensity ratio (RIR) valuesBy calculating them with Rietveld refinementSlide ‹#› of 20Scott A Speakman, Ph.D.
18 All calculations are more accurate if you use more peaks over a longer angular range If you use one or two peaks, you must assume:That there is no specimen displacement error when calculating lattice parametersThat there is no microstrain broadening when calculating crystallite sizeIf you use many peaks over a long angular range (for example, 7+ peaks over a 60° 2theta range), you can:Calculate and correct for specimen displacement when solving lattice parametersCalculate and account for microstrain broadening when calculating crystallite sizeImprove precision by one or two orders of magnitudeSlide ‹#› of 20Scott A Speakman, Ph.D.
19 There are different ways to extract peak information for quantitative analysis Numerical methods reduce the diffraction data to a list of discrete diffraction peaksThe peak list records the position, intensity, width and shape of each diffraction peakCalculations must be executed based on the peak list to produce information about the sampleFull pattern fitting methods refine a model of the sampleA diffraction pattern is calculated from a modelThe calculated and experimental diffraction patterns are comparedThe model is refined until the differences between the observed and calculated patterns are minimized.The Rietveld, LeBail, and Pawley fitting methods use different models to produce the calculated patternSlide ‹#› of 20Scott A Speakman, Ph.D.
20 A peak list for empirical analysis can be generated in different ways The diffraction data are reduced to a list of diffraction peaksPeak searchAnalysis of the second derivative of diffraction data is used to identify likely diffraction peaksPeak information is extracted by fitting a parabola around a minimum in the second derivativeThis method is fast but the peak information lacks precisionProfile fittingEach diffraction peak is fit independently with an equationThe sum of the profile fits recreates the experimental dataPeak information is extracted from the profile fit equationThis method provides the most precise peak informationSlide ‹#› of 20Scott A Speakman, Ph.D.
21 Profile Fitting produces precise peak positions, widths, heights, and areas with statistically valid estimates28.529.029.530.02q(deg.)Intensity (a.u.)Empirically fit experimental data with a series of equationsfit the diffraction peak using the profile functionThe profile function models the mixture of Gaussian and Lorentzian shapes that are typical of diffraction datafit background, usually as a polynomial functionthis helps to separate intensity in peak tails from backgroundTo extract information, operate explicitly on the equation rather than numerically on the raw dataSlide ‹#› of 20Scott A Speakman, Ph.D.
22 Diffraction peak lists are best reported using dhkl and relative intensity rather than 2q and absolute intensity.The peak position as 2q depends on instrumental characteristics such as wavelength.The peak position as dhkl is an intrinsic, instrument-independent, material property.Bragg’s Law is used to convert observed 2q positions to dhkl.The absolute intensity, i.e. the number of X rays observed in a given peak, can vary due to instrumental and experimental parameters.The relative intensities of the diffraction peaks should be instrument independent.To calculate relative intensity, divide the absolute intensity of every peak by the absolute intensity of the most intense peak, and then convert to a percentage. The most intense peak of a phase is therefore always called the “100% peak”.Peak areas are much more reliable than peak heights as a measure of intensity.Slide ‹#› of 20Scott A Speakman, Ph.D.
23 Calculations must be executed on the peak list to yield any information about the sample This peak list itself does not tell you anything about the sampleAdditional analysis must be done on the peak list to extract informationFrom the peak list you can determine:Phase composition: by comparison to a database of reference patternsSemi-quantitative phase composition: calculated from peak intensities for different phasesUnit cell lattice parameters: calculated from peak positionsCrystal system: determined by indexing observed peaks and systematic absencesCrystallite size and microstrain: calculated from peak widths and/or shapesA number of engineering indexes are also calculated from peak list informationSlide ‹#› of 20Scott A Speakman, Ph.D.
24 Full pattern fitting methods use different models to produce a calculated pattern The Rietveld method uses fundamental calculations from crystal structure models to produce the calculated diffraction patternAnalysis produces a refined crystal structure model for all phases in the samplePeak positions and intensities are constrained by the crystal structure modelCrystallite size, microstrain, and preferred orientation can be extracted from empirical models included in the refinementLe-Bail and Pawley fitting methods use unit cell models combined with empirical fitting of peak intensitiesAnalysis produces a refined unit cell model but does not immediate yield information about parameters related to peak intensitiesSlide ‹#› of 20Scott A Speakman, Ph.D.
25 Other analytical methods Total scattering methods (whole pattern fitting) attempts to model the entire diffraction pattern from first principal calculationsCalculations includeBragg diffraction peaks,diffuse scatter contributions to background,peak shapes based on diffractometer optics,peak shapes based on crystallite size, shape, defects, and microstrainPair distribution functional analysis uses Fourier analysis to produce an atomic pair density mapCan yield atomic structure information about non-crystalline, semi-crystalline, and highly disordered materialsSlide ‹#› of 20Scott A Speakman, Ph.D.
Your consent to our cookies if you continue to use this website.